STRUCTURAL CRYSTALLOGRAPHIC RELATION · PDF filestructural crystallographic relation between...
Embed Size (px)
Transcript of STRUCTURAL CRYSTALLOGRAPHIC RELATION · PDF filestructural crystallographic relation between...
STRUCTURAL CRYSTALLOGRAPHIC RELATIONBETWEEN SODIUM SULFATE AND POTASSIUM
SULFATE AND SOME OTHER SYNTHETICSULFATE MINERALSXT
M. E. Hrr,ux,l (Jniaersity oJ Michigan, Ann Arbor, Michigan
A study of the structural crystallographic relations between the following sulfate com-pounds has been made using r-ray methods as the main tooi: Na2SOrKzSOr, NasSOalir$Qa, KzSOr-LigSOr, KzSOc(NH4)rSO4 and NazSOr-(NHr)zSO+.
Aphthitalite, a sodium potassium sulfate mineral, has been prepared in the laboratoryfrom aqueous solutions as well as from fused melts of various sodium and potassium sulfateproportions. X-ray methods reveal that at high temperatures close to fusion, sodium sulfateand potassium sulfate are isomorphous and form a complete series of solid solutions. The
same synthetic mineral, prepared from aqueous solutions, has been found by *-ray inves-tigation and checked by chemical analysis to have a limited range of solid solution varyingbetween the ratios of lK:lNa to 5K:1Na when crystallized at 70'C. and limited to thealmost invariable ratio of 3K:lNa at room temperature.
X-ray powder data are given for LiKSOT and LiNaSOa, and also for the NHaKSOamember of the continuous series of crystaliine solid solution (NH4)2SO1-KrSO4. It isshown by the r-ray powder method that complete immiscibility exists between (NHn)rSO.
and NaaSOr at 70o C.For LiNaSOr ca:9.76 A+0.02, ao:7.64 A+0.02, space group P3Ic, Z:6, g. (deter-
mined):2.515, [email protected]) :2.527; basal twinningwith000lastwinningplaneiscommon.
The study of the structural relation between sodium sulfate and po-tassium sulfate is of particular interest in the field of crystallography be-cause of the fact that each compound occurs in more than one crystallo-graphic modification (polymorph) and that there has been some con-troversy as to whether there exists a solid solution relationship or iso-morphism, or both, between certain polymorphs of the two compounds.The existence of such solid solution or isomorphism, if any, is of specialinterest in structural crystallography because of the big difference inionic radii between sodium (0.98 A) and potassium (1.33 A;, *hich is
^ ^ . Requal to 0.35 A or 35.7/6 of the smaller ion (sodium). Sodium and po-tassium are not generally grouped together in isomorphous series. Po-tassium is usually grouped with rubidium and cesium but not with so-dium. Tutton (1922) in working out the isomorphous relationship be-tween the alkali sulfates excluded sodium sulfate from his series.
* Contribution from the Department of Mineralogy and Petrography, University ofMichigan, No. 176.
t Extracted from a thesis submitted in partial fulfillment of the requirements for thedegree of Doctor of Philosophy, University of Michigan, June 1952.
1 Present address: Dept. of Geology, Faculty of Science, Moharram Bey, Alexandria,Egvpt.
RELATION BETWEEN SODIUM AND POTASSIUM SULFATE tt9
Aphthitalite (or glaserite) has for a long time been assigned the com-position 3K2SO4 NazSOn or K3Na(SOr)2. It has been shown by a numberof investigators, Biicking (1889; Douglashall region in Germany), Teeple(1921; Searles Lake, California), Kurnakov, et, aI. (1936; Ural-Emba Dis-trict, Russia), and Kurnakov, et al. (1938; Permian Sea and the salt lakesof Western Kazakhstan, Russia), to be widespread in saline deposits ofIake basins. The mineral occurs also around volcanoes, e.g. Vesuvius,Scacchi (1875) and Bellanca (1942). Common among all these investi-gators, with the exception of Bellanca (1942), is the invariable composi-tion 3KrSOn'Na:SOr which they assigned to the mineral aphthitalite.
The composition and structure of aphthitalite have been the subjectmatter of argument and discussion since 1891. The problem is: Is thereany crystallographic relation between sodium sulfate and potassium sul-fate? Retgers (1891) stated that there is no isomorphism between sodiumsulfate and potassium sulfate. He considered aphthitalite as a doublesalt of the composition 3KrSOr*NazSOr. Van't Hofi (1903), on the otherhand, regarded aphthitalite as an isomorphous compound of the notclosely investigated hexagonal modifications of both components. Goss-ner (1904) considered aphthitalite as a binary compound of a constantchemical composition, NaK3(SOa)2. Van't Hoff and Barschall (1906)pointed to the existence of a series of solid solutions including the com-position NaKa(SOa)2. Druzhinin (1938), investigating the system NazSOr--KzSOa-HzO at the temperature of 25o C., considered aphthitalite as asolid solution of the definite chemical compound KsNa(SOn)z with NazSOrand reported that the compound permits substitution of Na for K withinthe range K/Na:2.44 to 3.00. Perrier and Bellanca (1940) and Bellanca(1942) using both thermal analysis technique and r-ray powder photo-graphs believe that the compound is not K3Na(SOr)z but rather KNaSOr.This forms solid solutions with KzSOa (up to 73 mol per cent total contentof the latter) and with Na:SOr (up to 75 mol per cent). Bredig (1942)states that aphthitalite should be considered simply as a solid solution ofthe high temperature forms of both potassium sulfate and sodium sulfate.Frondel (1950) gives the formula for aphthitalite as (KNa)sNa(SOr)2.Winchell (1951) considers aphthitalite, NaK3(SOa)r, as "a double salt-not a crystal solution." He mentions that the Na:K ratio seems to varyf rom about 1:4 to about 1:1.
Sodium sulfate exists in five polymorphous modifications: I, (II), III,(IV), and V. Using the x-ray powder method, Kracek and Ksanda(1930) showed that NazSOa I is stable above 240o C., Na2SO4 III ismetastable below 185o C. but inert when dry at ordinary temperatures,and NazSOe V is stable at ordinary temperatures. Polymorphs II and IVare unstable at ordinary pressure. NazSOr V is equivalent to the natu-
120 M. E. HILMY
rally occurring mineral thenardite, a rare salt lake deposit and also found
near some volcanoes.Potassium sulfate exists in two polymorphous modifications, namely:
(1) a high-temperature modification, called alpha-K2SOn, stable above
590' C. and is uniaxial negative, and (2) a low-temperature modification
called beta-KzSOa, stable at room temperature, orthorhombic, with the
space group Pmcn. Arcanite is the name of the mineral having the com-position KrSOr (equivalent to beta-KzSOr) and is said to be of very rare
occurrence (Frondel, 1950).Table 1 is a summary of the crystallographic data of the various sul-
fates mentioned above.
5 . 7 1J . t l
/ . J J
1. Calculated lrom data of Kracek and Ksanda (1930).2. Frevel (1940).3. Zachariassen and Zi.egler (1932).4. Bredig (1942).5. Strukturbericht (1937).6. Gossner (1928).7. Bellanca (1942).
Tna Rur,arroN BETwEEN Sopruu Sur,r'erB axp
The System NarSOa-KzSO + (Fused' samFl,es)
Samples were prepared by fusing mixtures of Na2SO4 and KzSOr
ranging in molecular ratios from 4:t to 1 :4. These gave very similar pow-
der photographs, and it seems apparent that when crystallizing from a
melt, there is a continuous solid solution between the hexagonal forms
of NazSOe and KlSOr. The pure end members always invert to a lower
RELATION BETWEEN SODIUM AND POTASSIUM SULFATE r21
symmetry modification upon cooling. On the other hand, there is arange of compositions between the end members in which the hexagonalform of the solid solution is stable. On either side of this stable range, asthe end member is approached, the originally formed solid solution un-mixes, yielding the pure end member, which inverts on cooling, and astable solid solution phase containing a lower percentage of the end mem-ber than was present in the melt.
The limits of this range in which the solid solution is stable are difficultto determine in samples prepared from melts. The material is so finegrained, and the variation in refractive indices so slight, that optical dif-ferentiation of a pure end member and a solid solution close to that endmember is impractical. The r-ray powder photographs of samples ap-proaching the end members in composition show increasing evidence of aphase consisting of the inverted end member. But in the range of 3: 1 to1:3, or even 4:t to l:4, this unmixing and inversion is negligible. Thisdifficulty in establishing definite limits for the stable range in materialprepared by fusion is not encountered when using single crystals pre-pared from solution. These are discussed later.
The lattice constants, ao and co, for some members of this high-tem-perature solid solution series of aphthitalite, have been determined fromthe corresponding powder photographs. These are given, together withthe published data on NazSOr I (calculated from data of Kracek andKsanda, 1930) and a-KzSOr (Bredig, 1942), in Table 2. This table showsclearly the increase in the unit cell dimensions as the result of the sub-stitution of potassium for sodium.
NazSOr I NarK
5 .397 .25
5. 507 .26s
5 . 7107 . 85
Thin sections and crushed fragments showed aphthitalite to be uni-axial positive. The values of co and e increase with higher content of po-tassium. They range from 1.485 toI.493for
122 M. E. HILMT/
Na+K) to 2.7 | (f or NaKa) with an experimental error of t 0'01. Winchell
(1951) gives the specific gravity ol2.7 f.or aphthitalite of the composition
NaKr(SOa)2. Gossner (1923) gave the value of 2.697 f.or the same com-
position. The specific gravity of aphthitalite from Vesuvius was repo